11.modelling tensile behaviour of stir cast aluminium matrix composites (am cs) using factorial design of experimentsDocument Transcript
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 Modelling Tensile Behaviour of Stir-cast Aluminium Matrix Composites (AMCs) Using Factorial Design of Experiments Indumati B. Deshmanya, Dr. GK Purohit Department of Mechanical Engineering, PDA College of Engineering Gulbarga, India E-mail: *firstname.lastname@example.org, email@example.comAbstractAluminium based metal matrix composites (MMCs) with ceramic reinforcement are finding extensiveapplications in aerospace, automobile, agricultural farm machinery and other areas which demandcombination of properties such as high strength, stiffness, wear resistance, high temperature resistance, etc.In particular, components comprising Al7075 alloy matrix, reinforced with alumina (Al2O3) particulates, arereported to excel their monolithic counterparts. Liquid metal route and powder metallurgy are the mostwidely used fabrication techniques to produce these MMCs. The former has advantages such as easyadaptability, low cost and possibility of subjecting the cast components to secondary processes like forging,rolling and extrusion for producing the final components. This paper presents the details of developing amathematical model to predict the tensile behavior like ultimate tensile strength (UTS) and percentageelongation of the as-cast Al7075/Al2O3 in terms of size and % fraction of Al2O3, holding temperature andholding time; using factorial design of experiments (DoE). Adequacy of the models was tested usingFisher’s F-test. UTS of the composite was increased by 20%compared to that of matrix and % elongationwas reduced by around 30%.Keywords: MMC, UTS, % elongation, Design of experiments, Modelling.1. IntroductionAluminium metal matrix composites (MMCs) with 7xxx alloy as matrix reinforced with ceramic particlesare finding application in aerospace, automobile and farm machinery equipment because of their improvedmechanical and tribological properties [1-6]. In particular, Al2O3 particles mixed with Al7075 matrix inappropriate proportions are reported to exhibit improved tensile properties because of the higher modulusof elasticity and strength of the alumina . Out of the available methods of producing these composites,stir casting route is most promising and economical for synthesizing the particle reinforced AMCs and isnot only simple, but is easy to obtain shape castings [8,9]. It is important to understand the processparameters that bring about the enhancement in their behaviour. However, conventionally, this requiresconducting costly and time consuming experiments. Alternately, we can predict the influence of processparameters accurately, and to develop composites possessing desirable mechanical properties variousmodelling methods are available [10-13]. This paper presents one such methodology called rotatable centralcomposite design (CCD), which is a multi-parameter based, multiple response analysis modellingtechnique . It is not only fast, economical and very effective in assessing the effect of individualparameters, but also helps in predicting the interaction effects of the parameters. Hence, in this work anattempt is made to predict the effect of reinforcement size, %weight fraction of reinforcement, holdingtemperature and holding time on the ultimate tensile strength and %elongation of a stir-cast Al7075/Al2O3composite system using CCD. The adequacy of the models is checked by Fisher’s-F ratio and the analysisof variance is employed to evaluate the effect of parameters.2. MaterialsAl7075 matrix reinforced with varying sizes of Al2O3 particles were used to produce composites using stircasting. Tables 1 and 2 present the important properties of the matrix material. Table 3 gives the range ofthe four most influential process parameters, viz. size of reinforcement particles (D), weight fraction ofreinforcement (W), holding temperature (T) and holding time (t). 5
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 20123. Experimental ProgramRotatable central composite design was used to produce the castings [15-17]. Figs. 1 and 2 show theschematic diagram and close-up view of stir casting process. The details of the process are explainedelsewhere . A total of 31 castings comprising 16 (=24) factorial points, 8 star points and 7 central pointswere produced by adapting the CCD as per Table 4. The castings were produced using randomness to avoidthe entry of systematic errors in experimentation. Tensile tests were performed on samples extracted fromdefect-free regions of the castings at a rate of 8.33×10-4 s-1 as per  and a minimum of 3 specimens weretested in each case. The average values of UTS and %E are presented in Table 4.4. Results and DiscussionThe maximum value of UTS obtained was 289MPa; minimum was 262MPa and the mean was at 273MPa,whereas %E obtained was in the range of 14.8% to 9.25% with the average at 11.3%. It is noticed thatintroduction of Al2O3 particulates could result in 20% increase in matrix UTS and decreased the %E byaround 30%; implying that composites with enhanced strength can be produced by stir-casting. However,one has to sacrifice the ductility. Similar observations have been made by many researchers [9,19-20].Second order relations were obtained by regression analysis and are presented in equations (1) and (2) forUTS and %E, respectively. UTS=270.29-3.63D+3.21W+2.36T+3.126t+0.768D2+2.643W2+0.518T2-0.106t2-0.437DW-0.313DT+ 0.563Dt-0.063Wt+0.937Tt (1) %E=10.508+0.396D-0.421W-0.0413T-0.453t+0.386D2+0.220W2+0.126T2+0.301t2-0.049DW-0.093DT +0.056Dt-0.21WT+0.363Wt+0.277Tt (2)Table 5 shows the result of the analyses of variance and it is noticed that, in both the cases, experimentalvalues of F-ratios are higher than that from the table; indicating that the two models are adequate. Also, R2and Radj2 values indicate that the models can be used to predict the responses with 99% confidence level.Hence, the models can be effectively used in predicting the UTS and %E, knowing the composition ofAl7075/Al2O3 MMCs.It is observed from equation (1) that as the size of reinforcement (D) increases UTS decreases. D affectsUTS independently as well as in combination with weight% and holding temperature. On the other hand, W,T and t contribute positively. Interestingly, the effect of these parameters on elongation is exactly reversedas shown in equation (2). Thus UTS of composites is observed to be 20% enhanced and elongation reducedby nearly 30% compared to the matrix material. Similar observations are recorded by many researchers[19-22]. Leisk and Saigal  have shown that further enhancement in tensile strength is possible bysubjecting the composites to heat treatment. However, this claim is to be confirmed for Al7075/Al2O3composites. All these aspects can be systematically exploited in developing the AMCs possessing desiredtensile strength and %elongation.5. ConclusionBased on the experimental work, following conclusions are drawn. 1 Rotatable, central composite design can be successfully used to model the tensile behaviour of AMCs 2 Mathematical models for UTS and %elongation are adequate and will predict the values with 99% confidence. 3 UTS and %elongation show reverse trends as far as influence of the process parameters are concerned. 4 UTS of the Al7075/Al2O3 MMCs increased by 20%compared to that of matrix and % elongation was reduced by around 30%.6. References Surappa M.K. (2003). Aluminium matrix composites: Challenges and Opportunities. Sadhana, 28 Parts 1 & 2, 319-344. 6
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 Ibrahim I.A, Mohamed F.A, Lavernia E.J. (1991). Particulate reinforced metal matrix composites- a review. Journal of Material Science, 26, 1137-1156. Nikhilesh Chawla, Yu-Lin Shen. (2001). Mechanical behaviour of particulate reinforced metal matrix composites. Advanced Engineering Materials, 3, 6, 357-370. Daoud A, Reif W, Rohatgi P. (2003). Microstructure and tensile properties of extruded 7475 AL-Al2O3 particulate composites. ECCM13, Sweden, 1201. Ceschini L, Minak G, Morri A. (2009). Forging of the AA2618/20 Vol. % Al2O3p composite: Effects on microstructure and tensile properties. Composites Science and Technology, 69, 1783-1789. Mallik, B., et al (2006). Effect of particle content on the mechanical behaviour of aluminium-based metal matrix composites (AMMC). Indian Foundry Journal, 52, 35-42. Hashim J, Looney L, Hashmi M. S. J. (1999). Metal matrix composites: production by the stir casting method. Journal of Materials Processing Technology, 92-93, 1- 7. Ceschini L, Minak G, Morri A. (2006). Tensile and fatigue properties of the AA6061/20 vol. % Al2O3p and AA7005/10 Vol. % Al2O3p composites. Composites Science and Technology, Vol. 66, 333-342 Gupta M, Lai M.O, Lim C.Y.H. (2006). Development of a novel hybrid aluminium-based composite with enhanced properties. Journal Material Processing Technology, Vol. 176, No. 1-3, 191-199. Sahin Y. (2003). Wear behavior of aluminium alloy and its composites reinforced by SiC particles using statistical analysis. Materials and Design, 24, 95-103. Yilmaz O, Buytoz S. (2001). Abrasive wear of Al2O3-reinforced aluminium-based MMCs. Composite Science and Technology, 61, 2381-2392. Mondal D.P, Das S. (2006). High stress abrasive wear behavior of aluminium hard particle composites: Effect of experimental parameters, particle size and volume fraction. Tribology International, 39, 470-478. Chawla N, Chawla K.K. (2006). Microstructural e-based modeling of the deformation behavior of particle reinforced metal matrix composites. Journal of Material Science and Technology, (41) 913-925. Deshmanya Indumati B, Purohit G.K. (2011). Studies on modelling of aluminium matrix composites (AMCs)-A Review. ICAM 2011, Joint International Conference on Advanced Materials. 144-145. Cochran W.G, Cox G M. (1992). Experimental Design, John Wiley, New York. Montgomery D. C. (2009). Design and Analysis of Experiments. John Wiley, New York. Adler Y.P, Markov E. V, Granovsky Y.V. (1975). The design of experiments to find optimal conditions. MIR Pub., Moscow. Deshmanya, Indumati B, Purohit G.K. (2011). Modelling of impact strength and hardness of Al2O3 – reinforced Al-7075 composites. International Journal of Industrial Engineering Practice, Vol. 3, Issue 1, 61-66. Doel T. J. A, Bowen P. (1996). Tensile properties of particulate-reinforced metal matrix composites. Composites Part A: Applied Science and Manufacturing, 27, 655-665. Srivatsan T.S. (1996). Microstructure tensile properties and fracture behaviour of Al2O3 particulate-reinforced aluminium alloy metal matrix composites. Journal of Materials Science, 31, 1375. Seah K. H. W, Sharma S. C, Girish B.M. (2001). Mechanical properties of as- cast and heat-treated ZA-27/graphite particulate composites. Composite: part A. 28A 251-6 Composites Science and Technology, 61, 2381. Abis S. (1989). Characterization of an aluminium alloy/alumina metal matrix composites. Journal of Composite Science and Technology, 35, 1-19. Leisk G, Saigal A. (1995). Taguchi analysis of heat treatment variables on the mechanical behaviour 7
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 of alumina /aluminium metal matrix composites. Composites Engineering, 5, 2, 129-142.Table 1: Chemical Composition of Al7075 Cr Cu Mg Zn Al Density g/cc at 20°C 0.22 1.60 2.80 5.50 Balance 2.89Table 2: Details of other important properties of Al7075 UTS Yield Strength Elongation Hardness Thermal Conductivity Elect. Resistivity 2 MPa MPa % VHN Cal/Cm /Cm/°C at 25°C µΩ-Cm at 20°C 228 103 17 79 0.29 5.74Table 3: Coded values of as-cast input variables at different levelsCoded Input Units Lower level Middle Upper levelvalues parameters Notation -2 -1 0 +1 +2 X1 Size of Al2O3 D µm 36 45 54 63 72 X2 % Wt of W --- 5 7.5 10 12.5 15 Al2O3 X3 Holding T 150 237 325 413 500 °C Temperature X4 Holding Time t Hrs 1 2 3 4 5 8
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 Table 5: Analysis of Variance (ANOVA) Particulars Source DF SS MS F R2 Radj2 I & II 14 455.438 32.531 Order Terms UTS Lack of Fit 10 885.07 3.571 9.11 98.42 98.18 Residual Error 6 21.427 Total 30 1361.935 36.102 9.11 98.42 98.18 2 Source DF SS MS F R Radj2 I & II 23.489 1.677 14 Frame Order Terms Driving motor Lack of Fit 42.54 Stirrer Rod 0.0198 84.52 99.81 99.79 % Elongation 10 Ball Bearing Residual Error 0.1191 6 Stirrer Blade Total 30 66.148 1.6968 84.52 99.81 99.79 Crucible Note: From Table; F14,6,0.05 = 4.07 (i.e. Fmodel > Ftable). Hence the model is adequate. Holding Furnace Figure 1: Schematic diagram showing components of stir-casting process. The stirrer is a servomotor operated ceramic coated stainless steel rod. 10
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 Figure 2:Close-up view of the stir-casting set-up. Al2O3 particulates of various sizes are added to the melt at 730°C which is continuously stirred using a motorized stirrer made of ceramic coated stainless steel rod. 11
International Journals Call for PaperThe IISTE, a U.S. publisher, is currently hosting the academic journals listed below. The peer review process of the following journalsusually takes LESS THAN 14 business days and IISTE usually publishes a qualified article within 30 days. Authors shouldsend their full paper to the following email address. More information can be found in the IISTE website : www.iiste.orgBusiness, Economics, Finance and Management PAPER SUBMISSION EMAILEuropean Journal of Business and Management EJBM@iiste.orgResearch Journal of Finance and Accounting RJFA@iiste.orgJournal of Economics and Sustainable Development JESD@iiste.orgInformation and Knowledge Management IKM@iiste.orgDeveloping Country Studies DCS@iiste.orgIndustrial Engineering Letters IEL@iiste.orgPhysical Sciences, Mathematics and Chemistry PAPER SUBMISSION EMAILJournal of Natural Sciences Research JNSR@iiste.orgChemistry and Materials Research CMR@iiste.orgMathematical Theory and Modeling MTM@iiste.orgAdvances in Physics Theories and Applications APTA@iiste.orgChemical and Process Engineering Research CPER@iiste.orgEngineering, Technology and Systems PAPER SUBMISSION EMAILComputer Engineering and Intelligent Systems CEIS@iiste.orgInnovative Systems Design and Engineering ISDE@iiste.orgJournal of Energy Technologies and Policy JETP@iiste.orgInformation and Knowledge Management IKM@iiste.orgControl Theory and Informatics CTI@iiste.orgJournal of Information Engineering and Applications JIEA@iiste.orgIndustrial Engineering Letters IEL@iiste.orgNetwork and Complex Systems NCS@iiste.orgEnvironment, Civil, Materials Sciences PAPER SUBMISSION EMAILJournal of Environment and Earth Science JEES@iiste.orgCivil and Environmental Research CER@iiste.orgJournal of Natural Sciences Research JNSR@iiste.orgCivil and Environmental Research CER@iiste.orgLife Science, Food and Medical Sciences PAPER SUBMISSION EMAILJournal of Natural Sciences Research JNSR@iiste.orgJournal of Biology, Agriculture and Healthcare JBAH@iiste.orgFood Science and Quality Management FSQM@iiste.orgChemistry and Materials Research CMR@iiste.orgEducation, and other Social Sciences PAPER SUBMISSION EMAILJournal of Education and Practice JEP@iiste.orgJournal of Law, Policy and Globalization JLPG@iiste.org Global knowledge sharing:New Media and Mass Communication NMMC@iiste.org EBSCO, Index Copernicus, UlrichsJournal of Energy Technologies and Policy JETP@iiste.org Periodicals Directory, JournalTOCS, PKPHistorical Research Letter HRL@iiste.org Open Archives Harvester, Bielefeld Academic Search Engine, ElektronischePublic Policy and Administration Research PPAR@iiste.org Zeitschriftenbibliothek EZB, Open J-Gate,International Affairs and Global Strategy IAGS@iiste.org OCLC WorldCat, Universe Digtial Library ,Research on Humanities and Social Sciences RHSS@iiste.org NewJour, Google Scholar.Developing Country Studies DCS@iiste.org IISTE is member of CrossRef. All journalsArts and Design Studies ADS@iiste.org have high IC Impact Factor Values (ICV).